#------------------------------------------------------------------------------
#$Date: 2016-03-25 23:21:01 +0200 (Fri, 25 Mar 2016) $
#$Revision: 180035 $
#$URL: svn://www.crystallography.net/cod/cif/7/03/29/7032977.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7032977
loop_
_publ_author_name
'Tian, Ai-xiang'
'Ning, Ya-li'
'Ying, Jun'
'Hou, Xue'
'Li, Tian-jiao'
'Wang, Xiu-li'
_publ_section_title
;
 Three multi-nuclear clusters and one infinite chain induced by a pendant
 4-butyl-1H-pyrazole ligand for modification of Keggin anions.
;
_journal_issue                   1
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              386
_journal_page_last               394
_journal_paper_doi               10.1039/c4dt02821j
_journal_volume                  44
_journal_year                    2015
_chemical_formula_sum            'C28 H56 Ag5 Mo24 N8 O86 P2'
_chemical_formula_weight         4785
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                94.672(5)
_cell_angle_beta                 107.070(5)
_cell_angle_gamma                110.939(5)
_cell_formula_units_Z            1
_cell_length_a                   11.928(5)
_cell_length_b                   12.117(5)
_cell_length_c                   18.608(5)
_cell_measurement_temperature    293(2)
_cell_volume                     2348.3(15)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.990
_diffrn_measured_fraction_theta_max 0.990
_diffrn_measurement_device_type  'Bruker P4'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71069
_diffrn_reflns_av_R_equivalents  0.0122
_diffrn_reflns_av_sigmaI/netI    0.0236
_diffrn_reflns_limit_h_max       12
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_k_max       11
_diffrn_reflns_limit_k_min       -14
_diffrn_reflns_limit_l_max       22
_diffrn_reflns_limit_l_min       -18
_diffrn_reflns_number            11764
_diffrn_reflns_theta_full        25.00
_diffrn_reflns_theta_max         25.00
_diffrn_reflns_theta_min         1.89
_diffrn_standards_decay_%        none
_exptl_absorpt_coefficient_mu    4.255
_exptl_absorpt_correction_T_max  0.600
_exptl_absorpt_correction_T_min  0.494
_exptl_absorpt_correction_type   numerical
_exptl_absorpt_process_details   'ABSCOR by T.Higashi    8  March, 1995'
_exptl_crystal_colour            orange
_exptl_crystal_density_diffrn    3.375
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             2229
_exptl_crystal_size_max          0.18
_exptl_crystal_size_mid          0.14
_exptl_crystal_size_min          0.12
_refine_diff_density_max         2.429
_refine_diff_density_min         -1.142
_refine_diff_density_rms         0.160
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   0.982
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     686
_refine_ls_number_reflns         8204
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      0.982
_refine_ls_R_factor_all          0.0404
_refine_ls_R_factor_gt           0.0330
_refine_ls_shift/su_max          0.026
_refine_ls_shift/su_mean         0.001
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0490P)²+17.7730P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0894
_refine_ls_wR_factor_ref         0.0930
_reflns_number_gt                7063
_reflns_number_total             8287
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            c4dt02821j2.cif
_cod_data_source_block           compound-4
_cod_depositor_comments
'Adding full bibliography for 7032974--7032977.cif.'
_cod_original_sg_symbol_H-M      P-1
_cod_database_code               7032977
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
P1 P 0.87958(13) 0.70294(12) 1.24011(8) 0.0120(3) Uani 1 1 d .
Mo1 Mo 1.00578(5) 0.98751(5) 1.36797(3) 0.02258(13) Uani 1 1 d .
Mo2 Mo 0.75751(6) 0.42711(5) 1.10473(3) 0.02807(14) Uani 1 1 d .
Mo3 Mo 0.60908(5) 0.46197(5) 1.24840(3) 0.02576(14) Uani 1 1 d .
Mo4 Mo 1.18884(5) 0.70114(5) 1.31497(3) 0.02618(14) Uani 1 1 d .
Mo5 Mo 0.93089(5) 0.45571(5) 1.30942(3) 0.02299(13) Uani 1 1 d .
Mo6 Mo 0.71439(5) 0.73584(5) 1.36596(3) 0.02197(13) Uani 1 1 d .
Mo7 Mo 0.84788(6) 0.96186(5) 1.17829(3) 0.02773(14) Uani 1 1 d .
Mo8 Mo 1.14126(5) 0.95471(5) 1.23433(3) 0.02639(14) Uani 1 1 d .
Mo9 Mo 1.03076(5) 0.71903(5) 1.43721(3) 0.02384(13) Uani 1 1 d .
Mo10 Mo 0.73692(6) 0.67786(6) 1.04029(3) 0.03042(15) Uani 1 1 d .
Mo11 Mo 0.56820(5) 0.69780(6) 1.17364(3) 0.02826(14) Uani 1 1 d .
Mo12 Mo 1.02592(6) 0.65692(6) 1.10757(3) 0.03012(15) Uani 1 1 d .
O1 O 0.7500(4) 0.6655(3) 1.2521(2) 0.0158(8) Uani 1 1 d .
O1W O 1.3923(6) 1.0707(6) 1.4400(4) 0.0609(17) Uani 1 1 d .
O2 O 0.8595(4) 0.6427(3) 1.1586(2) 0.0171(8) Uani 1 1 d .
O2W O 1.5315(6) 0.9467(6) 1.4017(4) 0.0586(17) Uani 1 1 d .
O3 O 0.9674(4) 0.6622(3) 1.2995(2) 0.0159(8) Uani 1 1 d .
O4 O 0.9413(4) 0.8405(3) 1.2501(2) 0.0161(8) Uani 1 1 d .
O5 O 0.6557(5) 0.6809(5) 0.9513(3) 0.0381(12) Uani 1 1 d .
O6 O 1.1258(5) 0.6568(4) 1.0600(3) 0.0338(11) Uani 1 1 d .
O7 O 1.3394(4) 0.7098(4) 1.3347(3) 0.0331(11) Uani 1 1 d .
O8 O 0.8942(5) 0.6846(4) 1.0290(3) 0.0299(10) Uani 1 1 d .
O9 O 0.4313(4) 0.7136(4) 1.1304(3) 0.0340(11) Uani 1 1 d .
O10 O 0.5888(4) 0.7473(4) 1.2818(2) 0.0241(9) Uani 1 1 d .
O11 O 0.6994(5) 0.2836(4) 1.0584(3) 0.0356(12) Uani 1 1 d .
O12 O 0.9265(4) 0.3224(4) 1.3287(3) 0.0305(11) Uani 1 1 d .
O13 O 1.0512(5) 1.1023(4) 1.4401(3) 0.0309(11) Uani 1 1 d .
O14 O 1.0889(4) 0.8298(4) 1.1520(3) 0.0267(10) Uani 1 1 d .
O15 O 0.6144(4) 0.6546(4) 1.0911(2) 0.0265(10) Uani 1 1 d .
O16 O 0.6188(4) 0.5589(4) 1.3365(2) 0.0232(9) Uani 1 1 d .
O17 O 0.6665(5) 0.7650(4) 1.4387(3) 0.0304(11) Uani 1 1 d .
O18 O 0.8033(5) 1.0632(4) 1.1366(3) 0.0339(11) Uani 1 1 d .
O19 O 0.9125(4) 1.0408(4) 1.2831(3) 0.0243(9) Uani 1 1 d .
O20 O 1.1026(4) 0.5307(4) 1.3169(2) 0.0228(9) Uani 1 1 d .
O21 O 1.0938(5) 0.7466(5) 1.5335(2) 0.0303(11) Uani 1 1 d .
O22 O 1.1156(4) 0.6476(4) 1.2050(2) 0.0263(10) Uani 1 1 d .
O23 O 1.1423(4) 1.0374(4) 1.3310(3) 0.0255(10) Uani 1 1 d .
O24 O 0.6902(5) 0.5007(4) 1.0271(2) 0.0293(10) Uani 1 1 d .
O25 O 0.6449(4) 0.4258(4) 1.1557(2) 0.0246(9) Uani 1 1 d .
O26 O 0.7593(4) 0.4440(4) 1.3010(2) 0.0224(9) Uani 1 1 d .
O27 O 0.4946(4) 0.3304(4) 1.2454(3) 0.0323(11) Uani 1 1 d .
O28 O 1.1858(4) 0.7355(4) 1.4150(2) 0.0238(9) Uani 1 1 d .
O29 O 0.5063(4) 0.5376(4) 1.1878(2) 0.0239(9) Uani 1 1 d .
O30 O 0.6954(4) 0.8571(4) 1.1872(3) 0.0245(10) Uani 1 1 d .
O31 O 1.2793(5) 1.0551(4) 1.2332(3) 0.0356(12) Uani 1 1 d .
O32 O 0.8691(4) 0.4226(4) 1.2025(2) 0.0240(9) Uani 1 1 d .
O33 O 0.8365(4) 0.8849(4) 1.3677(2) 0.0222(9) Uani 1 1 d .
O34 O 1.2015(4) 0.8536(4) 1.2984(3) 0.0265(10) Uani 1 1 d .
O35 O 0.9844(4) 0.5485(4) 1.4148(2) 0.0228(9) Uani 1 1 d .
O36 O 1.0601(4) 0.8768(4) 1.4164(2) 0.0219(9) Uani 1 1 d .
O37 O 0.8598(4) 0.6957(4) 1.4169(2) 0.0212(9) Uani 1 1 d .
O38 O 0.9166(5) 0.4933(4) 1.0817(3) 0.0297(10) Uani 1 1 d .
O39 O 0.8106(4) 0.8383(4) 1.0905(2) 0.0258(10) Uani 1 1 d .
O40 O 1.0243(4) 1.0184(4) 1.1820(3) 0.0253(10) Uani 1 1 d .
Ag1 Ag 1.05243(6) 0.75291(7) 0.92574(4) 0.05277(19) Uani 1 1 d .
Ag2 Ag 1.0000 1.0000 1.0000 0.0904(5) Uani 1 2 d S
Ag3 Ag 0.76593(7) 0.48226(6) 0.91529(3) 0.04434(16) Uani 1 1 d .
C1 C 1.3180(7) 0.9179(7) 1.0536(4) 0.0372(17) Uani 1 1 d .
H1A H 1.3548 0.8625 1.0507 0.045 Uiso 1 1 calc R
C2 C 1.3813(6) 1.0313(5) 1.0952(3) 0.0215(13) Uani 1 1 d .
C3 C 1.2949(9) 1.0776(7) 1.0851(4) 0.044(2) Uani 1 1 d .
H3A H 1.3113 1.1557 1.1077 0.053 Uiso 1 1 calc R
C4 C 1.5148(8) 1.0928(8) 1.1451(5) 0.049(2) Uani 1 1 d .
H4A H 1.5348 1.1781 1.1602 0.059 Uiso 1 1 calc R
H4B H 1.5694 1.0853 1.1170 0.059 Uiso 1 1 calc R
C5 C 1.5424(7) 1.0405(7) 1.2166(5) 0.0410(19) Uani 1 1 d .
H5A H 1.4779 1.0334 1.2398 0.049 Uiso 1 1 calc R
H5B H 1.5402 0.9606 1.2030 0.049 Uiso 1 1 calc R
C6 C 1.6715(7) 1.1219(7) 1.2724(5) 0.0433(19) Uani 1 1 d .
H6A H 1.6687 1.1972 1.2920 0.052 Uiso 1 1 calc R
H6B H 1.7328 1.1404 1.2459 0.052 Uiso 1 1 calc R
C7 C 1.7139(6) 1.0676(7) 1.3366(4) 0.0319(16) Uani 1 1 d .
H7A H 1.7966 1.1230 1.3712 0.048 Uiso 1 1 calc R
H7B H 1.7194 0.9943 1.3175 0.048 Uiso 1 1 calc R
H7C H 1.6538 1.0498 1.3632 0.048 Uiso 1 1 calc R
C8 C 0.7055(6) 0.5461(6) 0.7460(4) 0.0291(15) Uani 1 1 d .
H8A H 0.6249 0.4831 0.7259 0.035 Uiso 1 1 calc R
C9 C 0.7547(5) 0.6296(5) 0.7074(3) 0.0165(12) Uani 1 1 d .
C10 C 0.8710(7) 0.7025(6) 0.7568(4) 0.0345(16) Uani 1 1 d .
H10A H 0.9279 0.7693 0.7463 0.041 Uiso 1 1 calc R
C11 C 0.6925(9) 0.6469(8) 0.6311(4) 0.046(2) Uani 1 1 d .
H11A H 0.6981 0.7291 0.6349 0.056 Uiso 1 1 calc R
H11B H 0.6027 0.5926 0.6119 0.056 Uiso 1 1 calc R
C12 C 0.7609(10) 0.6203(10) 0.5720(6) 0.079(4) Uani 1 1 d .
H12A H 0.7580 0.6720 0.5349 0.095 Uiso 1 1 calc R
H12B H 0.8499 0.6377 0.6001 0.095 Uiso 1 1 calc R
C13 C 0.6966(10) 0.4981(10) 0.5337(6) 0.076(3) Uani 1 1 d .
H13A H 0.6095 0.4821 0.5021 0.091 Uiso 1 1 calc R
H13B H 0.6936 0.4463 0.5708 0.091 Uiso 1 1 calc R
C14 C 0.7694(7) 0.4726(7) 0.4832(4) 0.0328(16) Uani 1 1 d .
H14A H 0.7280 0.3891 0.4574 0.049 Uiso 1 1 calc R
H14B H 0.8558 0.4899 0.5149 0.049 Uiso 1 1 calc R
H14C H 0.7699 0.5227 0.4458 0.049 Uiso 1 1 calc R
N1 N 1.1835(7) 0.9997(6) 1.0392(4) 0.0430(16) Uani 1 1 d .
N2 N 1.1999(6) 0.8960(6) 1.0185(3) 0.0349(14) Uani 1 1 d .
N3 N 0.8933(5) 0.6665(5) 0.8220(3) 0.0313(13) Uani 1 1 d .
N4 N 0.7862(5) 0.5656(5) 0.8150(3) 0.0272(12) Uani 1 1 d .
O3W O 1.5686(11) 1.2469(10) 1.3954(6) 0.120(3) Uiso 1 1 d .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ag Ag -0.8971 1.1015 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O4 P1 O2 109.4(2) . .
O4 P1 O3 109.4(2) . .
O2 P1 O3 109.5(2) . .
O4 P1 O1 109.8(2) . .
O2 P1 O1 109.6(2) . .
O3 P1 O1 109.1(2) . .
O13 Mo1 O23 102.0(2) . .
O13 Mo1 O36 103.4(2) . .
O23 Mo1 O36 92.49(19) . .
O13 Mo1 O19 100.7(2) . .
O23 Mo1 O19 87.3(2) . .
O36 Mo1 O19 155.43(18) . .
O13 Mo1 O33 101.6(2) . .
O23 Mo1 O33 156.18(18) . .
O36 Mo1 O33 85.30(19) . .
O19 Mo1 O33 85.09(18) . .
O13 Mo1 O4 171.6(2) . .
O23 Mo1 O4 73.72(16) . .
O36 Mo1 O4 84.13(16) . .
O19 Mo1 O4 72.21(16) . .
O33 Mo1 O4 82.46(16) . .
O11 Mo2 O25 103.3(2) . .
O11 Mo2 O24 102.2(2) . .
O25 Mo2 O24 94.9(2) . .
O11 Mo2 O32 101.1(2) . .
O25 Mo2 O32 85.64(19) . .
O24 Mo2 O32 155.91(19) . .
O11 Mo2 O38 100.1(2) . .
O25 Mo2 O38 155.90(19) . .
O24 Mo2 O38 85.9(2) . .
O32 Mo2 O38 84.1(2) . .
O11 Mo2 O2 171.3(2) . .
O25 Mo2 O2 84.99(17) . .
O24 Mo2 O2 74.15(17) . .
O32 Mo2 O2 81.92(16) . .
O38 Mo2 O2 72.03(16) . .
O27 Mo3 O26 102.8(2) . .
O27 Mo3 O16 101.1(2) . .
O26 Mo3 O16 92.38(19) . .
O27 Mo3 O25 101.9(2) . .
O26 Mo3 O25 85.69(19) . .
O16 Mo3 O25 156.84(19) . .
O27 Mo3 O29 100.5(2) . .
O26 Mo3 O29 156.38(18) . .
O16 Mo3 O29 87.24(19) . .
O25 Mo3 O29 85.49(19) . .
O27 Mo3 O1 170.99(19) . .
O26 Mo3 O1 85.20(17) . .
O16 Mo3 O1 74.10(16) . .
O25 Mo3 O1 82.74(16) . .
O29 Mo3 O1 71.96(16) . .
O7 Mo4 O34 103.8(2) . .
O7 Mo4 O28 101.0(2) . .
O34 Mo4 O28 92.7(2) . .
O7 Mo4 O22 103.0(2) . .
O34 Mo4 O22 86.5(2) . .
O28 Mo4 O22 155.41(19) . .
O7 Mo4 O20 99.3(2) . .
O34 Mo4 O20 156.69(19) . .
O28 Mo4 O20 86.18(19) . .
O22 Mo4 O20 84.99(19) . .
O7 Mo4 O3 170.2(2) . .
O34 Mo4 O3 85.03(17) . .
O28 Mo4 O3 73.95(16) . .
O22 Mo4 O3 81.51(16) . .
O20 Mo4 O3 72.28(15) . .
O12 Mo5 O32 102.4(2) . .
O12 Mo5 O20 100.1(2) . .
O32 Mo5 O20 93.94(19) . .
O12 Mo5 O26 102.5(2) . .
O32 Mo5 O26 85.47(19) . .
O20 Mo5 O26 157.02(18) . .
O12 Mo5 O35 99.9(2) . .
O32 Mo5 O35 157.22(18) . .
O20 Mo5 O35 86.76(19) . .
O26 Mo5 O35 85.15(17) . .
O12 Mo5 O3 170.90(19) . .
O32 Mo5 O3 85.15(16) . .
O20 Mo5 O3 74.03(16) . .
O26 Mo5 O3 83.04(16) . .
O35 Mo5 O3 73.14(15) . .
O17 Mo6 O33 103.7(2) . .
O17 Mo6 O10 101.7(2) . .
O33 Mo6 O10 92.85(19) . .
O17 Mo6 O37 102.3(2) . .
O33 Mo6 O37 86.06(19) . .
O10 Mo6 O37 155.58(18) . .
O17 Mo6 O16 99.2(2) . .
O33 Mo6 O16 156.45(18) . .
O10 Mo6 O16 87.74(19) . .
O37 Mo6 O16 83.82(18) . .
O17 Mo6 O1 170.6(2) . .
O33 Mo6 O1 84.98(16) . .
O10 Mo6 O1 73.87(16) . .
O37 Mo6 O1 81.73(15) . .
O16 Mo6 O1 72.57(15) . .
O18 Mo7 O30 102.0(2) . .
O18 Mo7 O19 100.2(2) . .
O30 Mo7 O19 92.10(19) . .
O18 Mo7 O40 100.7(2) . .
O30 Mo7 O40 157.06(19) . .
O19 Mo7 O40 87.37(19) . .
O18 Mo7 O39 102.6(2) . .
O30 Mo7 O39 85.85(19) . .
O19 Mo7 O39 157.00(19) . .
O40 Mo7 O39 85.78(19) . .
O18 Mo7 O4 171.5(2) . .
O30 Mo7 O4 84.56(16) . .
O19 Mo7 O4 73.86(16) . .
O40 Mo7 O4 73.25(16) . .
O39 Mo7 O4 83.14(16) . .
O31 Mo8 O14 104.8(2) . .
O31 Mo8 O40 101.5(2) . .
O14 Mo8 O40 93.5(2) . .
O31 Mo8 O34 100.9(2) . .
O14 Mo8 O34 86.3(2) . .
O40 Mo8 O34 156.92(19) . .
O31 Mo8 O23 97.7(2) . .
O14 Mo8 O23 156.95(19) . .
O40 Mo8 O23 86.86(19) . .
O34 Mo8 O23 84.47(19) . .
O31 Mo8 O4 169.5(2) . .
O14 Mo8 O4 85.11(17) . .
O40 Mo8 O4 74.06(17) . .
O34 Mo8 O4 82.95(17) . .
O23 Mo8 O4 72.83(15) . .
O21 Mo9 O37 104.3(2) . .
O21 Mo9 O35 99.6(2) . .
O37 Mo9 O35 91.22(19) . .
O21 Mo9 O36 102.8(2) . .
O37 Mo9 O36 87.17(18) . .
O35 Mo9 O36 157.17(18) . .
O21 Mo9 O28 98.0(2) . .
O37 Mo9 O28 157.64(18) . .
O35 Mo9 O28 86.33(18) . .
O36 Mo9 O28 86.58(19) . .
O21 Mo9 O3 169.47(19) . .
O37 Mo9 O3 84.58(16) . .
O35 Mo9 O3 74.26(15) . .
O36 Mo9 O3 82.92(16) . .
O28 Mo9 O3 73.35(15) . .
O5 Mo10 O39 103.3(2) . .
O5 Mo10 O15 103.0(2) . .
O39 Mo10 O15 87.04(19) . .
O5 Mo10 O8 100.8(2) . .
O39 Mo10 O8 92.4(2) . .
O15 Mo10 O8 155.62(19) . .
O5 Mo10 O24 98.7(2) . .
O39 Mo10 O24 157.95(19) . .
O15 Mo10 O24 86.7(2) . .
O8 Mo10 O24 84.7(2) . .
O5 Mo10 O2 169.6(2) . .
O39 Mo10 O2 85.58(17) . .
O15 Mo10 O2 82.42(16) . .
O8 Mo10 O2 73.24(16) . .
O24 Mo10 O2 72.65(16) . .
O9 Mo11 O15 103.3(2) . .
O9 Mo11 O29 101.6(2) . .
O15 Mo11 O29 92.6(2) . .
O9 Mo11 O30 102.3(2) . .
O15 Mo11 O30 86.20(19) . .
O29 Mo11 O30 155.70(18) . .
O9 Mo11 O10 99.4(2) . .
O15 Mo11 O10 157.00(19) . .
O29 Mo11 O10 86.34(19) . .
O30 Mo11 O10 85.48(19) . .
O9 Mo11 O1 170.5(2) . .
O15 Mo11 O1 85.01(17) . .
O29 Mo11 O1 72.99(16) . .
O30 Mo11 O1 82.73(16) . .
O10 Mo11 O1 72.69(15) . .
O6 Mo12 O22 102.0(2) . .
O6 Mo12 O38 100.9(2) . .
O22 Mo12 O38 93.4(2) . .
O6 Mo12 O14 101.8(2) . .
O22 Mo12 O14 84.72(19) . .
O38 Mo12 O14 157.11(19) . .
O6 Mo12 O8 100.4(2) . .
O22 Mo12 O8 156.83(19) . .
O38 Mo12 O8 88.0(2) . .
O14 Mo12 O8 85.07(19) . .
O6 Mo12 O2 172.0(2) . .
O22 Mo12 O2 84.85(17) . .
O38 Mo12 O2 74.26(17) . .
O14 Mo12 O2 82.85(16) . .
O8 Mo12 O2 73.27(16) . .
P1 O1 Mo11 125.1(2) . .
P1 O1 Mo6 126.1(2) . .
Mo11 O1 Mo6 89.22(13) . .
P1 O1 Mo3 126.0(2) . .
Mo11 O1 Mo3 89.53(13) . .
Mo6 O1 Mo3 89.32(13) . .
P1 O2 Mo12 125.6(2) . .
P1 O2 Mo10 125.2(2) . .
Mo12 O2 Mo10 90.09(13) . .
P1 O2 Mo2 125.7(2) . .
Mo12 O2 Mo2 89.28(13) . .
Mo10 O2 Mo2 89.57(13) . .
P1 O3 Mo5 125.8(2) . .
P1 O3 Mo9 126.0(2) . .
Mo5 O3 Mo9 89.96(13) . .
P1 O3 Mo4 125.6(2) . .
Mo5 O3 Mo4 89.00(13) . .
Mo9 O3 Mo4 88.87(13) . .
P1 O4 Mo7 126.0(2) . .
P1 O4 Mo8 126.1(2) . .
Mo7 O4 Mo8 89.11(13) . .
P1 O4 Mo1 125.5(2) . .
Mo7 O4 Mo1 89.16(13) . .
Mo8 O4 Mo1 89.19(13) . .
Mo12 O6 Ag3 117.4(2) . 2_767
Mo10 O8 Mo12 123.4(2) . .
Mo11 O9 Ag3 114.2(2) . 2_667
Mo6 O10 Mo11 124.2(2) . .
Mo8 O14 Mo12 151.1(3) . .
Mo11 O15 Mo10 150.9(3) . .
Mo3 O16 Mo6 123.9(2) . .
Mo7 O19 Mo1 124.7(2) . .
Mo5 O20 Mo4 124.7(2) . .
Mo12 O22 Mo4 153.1(3) . .
Mo1 O23 Mo8 124.2(2) . .
Mo2 O24 Mo10 123.6(2) . .
Mo2 O24 Ag3 111.5(2) . .
Mo10 O24 Ag3 95.61(18) . .
Mo2 O25 Mo3 151.6(2) . .
Mo3 O26 Mo5 150.2(2) . .
Mo4 O28 Mo9 123.8(2) . .
Mo11 O29 Mo3 125.5(2) . .
Mo7 O30 Mo11 151.5(3) . .
Mo5 O32 Mo2 152.3(3) . .
Mo6 O33 Mo1 151.9(2) . .
Mo4 O34 Mo8 149.8(3) . .
Mo9 O35 Mo5 122.6(2) . .
Mo1 O36 Mo9 152.1(2) . .
Mo9 O37 Mo6 149.6(2) . .
Mo12 O38 Mo2 124.4(2) . .
Mo10 O39 Mo7 150.1(2) . .
Mo8 O40 Mo7 123.6(2) . .
N3 Ag1 N2 159.0(2) . .
N1 Ag2 N1 179.999(3) . 2_777
N4 Ag3 O6 113.56(18) . 2_767
N4 Ag3 O24 140.72(18) . .
O6 Ag3 O24 105.13(15) 2_767 .
N4 Ag3 O9 109.12(18) . 2_667
O6 Ag3 O9 82.05(17) 2_767 2_667
O24 Ag3 O9 82.09(16) . 2_667
N2 C1 C2 111.0(7) . .
C3 C2 C1 105.2(7) . .
C3 C2 C4 125.2(7) . .
C1 C2 C4 129.5(7) . .
C2 C3 N1 110.9(7) . .
C2 C4 C5 111.7(6) . .
C6 C5 C4 109.0(7) . .
C5 C6 C7 112.1(7) . .
N4 C8 C9 110.9(6) . .
C10 C9 C8 105.0(6) . .
C10 C9 C11 126.0(7) . .
C8 C9 C11 128.7(7) . .
N3 C10 C9 110.4(6) . .
C9 C11 C12 110.2(6) . .
C13 C12 C11 109.1(9) . .
C12 C13 C14 108.2(9) . .
C3 N1 N2 106.4(7) . .
C3 N1 Ag2 134.2(6) . .
N2 N1 Ag2 119.3(5) . .
C1 N2 N1 106.4(6) . .
C1 N2 Ag1 132.0(5) . .
N1 N2 Ag1 120.3(5) . .
C10 N3 N4 107.2(6) . .
C10 N3 Ag1 128.3(5) . .
N4 N3 Ag1 124.2(4) . .
C8 N4 N3 106.5(6) . .
C8 N4 Ag3 131.6(5) . .
N3 N4 Ag3 121.4(4) . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
P1 O4 1.532(4) .
P1 O2 1.540(4) .
P1 O3 1.530(4) .
P1 O1 1.537(4) .
Mo1 O13 1.662(4) .
Mo1 O23 1.874(4) .
Mo1 O36 1.873(4) .
Mo1 O19 1.949(4) .
Mo1 O33 1.955(4) .
Mo1 O4 2.443(4) .
Mo2 O11 1.671(5) .
Mo2 O25 1.855(4) .
Mo2 O24 1.889(5) .
Mo2 O32 1.931(4) .
Mo2 O38 1.968(5) .
Mo2 O2 2.428(4) .
Mo3 O27 1.672(5) .
Mo3 O26 1.871(4) .
Mo3 O16 1.886(4) .
Mo3 O25 1.947(4) .
Mo3 O29 1.943(4) .
Mo3 O1 2.420(4) .
Mo4 O7 1.687(5) .
Mo4 O34 1.858(5) .
Mo4 O28 1.887(4) .
Mo4 O22 1.923(4) .
Mo4 O20 1.959(5) .
Mo4 O3 2.433(4) .
Mo5 O12 1.669(5) .
Mo5 O32 1.861(4) .
Mo5 O20 1.877(4) .
Mo5 O26 1.958(4) .
Mo5 O35 1.978(4) .
Mo5 O3 2.414(4) .
Mo6 O17 1.674(4) .
Mo6 O33 1.862(4) .
Mo6 O10 1.876(4) .
Mo6 O37 1.964(4) .
Mo6 O16 1.973(5) .
Mo6 O1 2.426(4) .
Mo7 O18 1.665(5) .
Mo7 O30 1.873(4) .
Mo7 O19 1.897(4) .
Mo7 O40 1.944(5) .
Mo7 O39 1.952(4) .
Mo7 O4 2.409(4) .
Mo8 O31 1.669(5) .
Mo8 O14 1.847(4) .
Mo8 O40 1.893(5) .
Mo8 O34 1.950(5) .
Mo8 O23 1.981(4) .
Mo8 O4 2.410(4) .
Mo9 O21 1.678(4) .
Mo9 O37 1.871(4) .
Mo9 O35 1.912(4) .
Mo9 O36 1.910(4) .
Mo9 O28 1.957(4) .
Mo9 O3 2.412(4) .
Mo10 O5 1.667(5) .
Mo10 O39 1.851(4) .
Mo10 O15 1.917(5) .
Mo10 O8 1.923(5) .
Mo10 O24 1.989(5) .
Mo10 O2 2.424(4) .
Mo11 O9 1.682(5) .
Mo11 O15 1.872(4) .
Mo11 O29 1.885(4) .
Mo11 O30 1.922(5) .
Mo11 O10 1.970(4) .
Mo11 O1 2.414(4) .
Mo12 O6 1.681(4) .
Mo12 O22 1.851(5) .
Mo12 O38 1.868(5) .
Mo12 O14 1.966(5) .
Mo12 O8 1.956(5) .
Mo12 O2 2.401(4) .
O6 Ag3 2.459(5) 2_767
O9 Ag3 2.529(5) 2_667
O24 Ag3 2.524(5) .
Ag1 N3 2.128(6) .
Ag1 N2 2.152(6) .
Ag2 N1 2.096(7) .
Ag2 N1 2.096(7) 2_777
Ag3 N4 2.227(6) .
Ag3 O6 2.459(5) 2_767
Ag3 O9 2.529(5) 2_667
C1 N2 1.282(10) .
C1 C2 1.341(10) .
C2 C3 1.315(11) .
C2 C4 1.458(10) .
C3 N1 1.301(11) .
C4 C5 1.520(12) .
C5 C6 1.493(11) .
C6 C7 1.459(11) .
C8 N4 1.301(9) .
C8 C9 1.351(9) .
C9 C10 1.340(9) .
C9 C11 1.466(9) .
C10 N3 1.308(9) .
C11 C12 1.625(15) .
C12 C13 1.409(15) .
C13 C14 1.534(14) .
N1 N2 1.381(9) .
N3 N4 1.379(8) .
